# ch06 ```CHAPTER 6
MECHANICAL PROPERTIES OF METALS
PROBLEM SOLUTIONS
Concepts of Stress and Strain
6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram), derive Equations 6.4a and 6.4b.
Solution
This problem asks that we derive Equations 6.4a and 6.4b, using mechanics of materials principles. In Figure
(a) below is shown a block element of material of cross-sectional area A that is subjected to a tensile force P. Also
represented is a plane that is oriented at an angle q referenced to the plane perpendicular to the tensile axis; the area
of this plane is A' = A/cos q. In addition, and the forces normal and parallel to this plane are labeled as P' and V',
respectively. Furthermore, on the left-hand side of this block element are shown force components that are tangential
and perpendicular to the inclined plane. In Figure (b) are shown the orientations of the applied stress s, the normal
stress to this plane s', as well as the shear stress t' taken parallel to this inclined plane. In addition, two coordinate
axis systems in represented in Figure (c): the primed x and y axes are referenced to the inclined plane, whereas the
unprimed x axis is taken parallel to the applied stress.
Normal and shear stresses are defin ed by Equations 6.1 and 6.3, respectively. However, we now chose to
express these stresses in terms (i.e., general terms) of normal and shear forces (P and V) as
s=
P
A
t =
V
A
For static equilibrium in the x' direction the following condition must be met:
å F x'
=0
which means that
P - P cos q = 0
Or that
P' = P cos q
Now it is possible to write an expression for the stress s' in terms of P' and A' using the above expression and the
relationship between A and A' [Figure (a)]:
s' =
=
P
A
P cos q
P
=
cos 2q
A
A
cos q
However, it is the case that P/A = s; and, after making this substitution into the above expression, we have Equation
6.4a--that is
2
s' = s cos q
Now, for static equilibrium in the y' direction, it is necessary that
åFy
=0
= - V + P sin q
Or
V' = P sin q
We now write an expression for t' as
t =
V
A
And, substitution of the above equation for V' and also the expression for A' gives
t' =
=
=
V
A
P sinq
A
cos q
P
sinq cos q
A
= s sinq cos q
which is just Equation 6.4b.
6.2 (a) Equations 6.4a and 6.4b are expressions for normal (σ ) and shear (τ ) stresses, respectively, as a
function of the applied tensile stress (σ) and the inclination angle of the plane on which these stresses are taken (θ
of Figure 6.4). Make a plot on which is presented the orientation parameters of these expressions (i.e., cos2 θ and
sin θ cos θ) versus θ.
(b) From this plot, at what angle of inclination is the normal stress a maximum?
(c) Also, at what inclination angle is the shear stress a maximum?
Solution
(a) Below are plotted curves of cos 2q (for s' ) and sin q cos q (for t') versus q.
(b) The maximum normal stress occurs at an inclination angle of 0°.
(c) The maximum shear stress occurs at an inclination angle of 45°.
Stress-Strain Behavior
6.3 A specimen of aluminum having a rectangular cross section 10 mm ´ 12.7 mm (0.4 in. ´ 0.5 in.) is
pulled in tension with 35,500 N (8000 lb f) force, producing only elastic deformation. Calculate the resulting
strain.
Solution
This problem calls for us to calculate the elastic strain that results for an aluminum specimen stressed in
tension. The cross-sectional area is just (10 mm) ´ (12.7 mm) = 127 mm2 (= 1.27 ´ 10-4 m2 = 0.20 in.2 ); also, the elastic
2
modulus for Al is given in Table 6.1 as 69 GPa (or 69 ´ 109 N/m ). Combining Equations 6.1 and 6.5 and solving for
the strain yields
e =
s
F
=
=
E
A0 E
(1.27 ´
35, 500 N
= 4.1 ´ 10 -3
m2 )(69 ´ 10 9 N/m2 )
10 -4
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 ´ 10 6 psi) and
an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile load of 2000 N
(450 lb f) is applied. Compute the maximum length of the specimen before deformation if the maximum allowable
elongation is 0.42 mm (0.0165 in.).
Solution
We are asked to compute the maximum length of a cylindrical titanium alloy specimen (before deformation)
that is deformed elastically in tension. For a cylindrical specimen
æ d ö2
A0 = pç 0 ÷
è 2 ø
where d 0 is the original diameter. Combining Equations 6.1, 6.2, and 6.5 and solving for l0 leads to
æ d ö2
Dl Ep ç 0 ÷
Dl Ep d02
Dl
Dl
Dl E
è2 ø
l0 =
=
=
=
=
s
F
e
F
4F
E
A0
=
(0.42 ´ 10 -3 m)(107 ´ 10 9 N / m2 ) (p) (3.8 ´ 10 -3 m) 2
(4)(2000 N)
= 0.255 m = 255 mm (10.0 in.)
6.5 A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm (0.8 in.) on an edge is
pulled in tension with a load of 89,000 N (20,000 lb f), and experiences an elongation of 0.10 mm (4.0 ´ 10 -3 in.).
Assuming that the deformation is entirely elastic, calculate the elastic modulus of the steel.
Solution
This problem asks us to compute the elastic modulus of steel. For a square cross-section, A0 = b02 , where
b 0 is the edge length. Combining Equations 6.1, 6.2, and 6.5 and solving for E, leads to
F
s
A0
Fl
E =
=
= 20
Dl
e
b0D l
l0
=
(89, 000 N) (100 ´ 10 -3 m)
(20 ´ 10 -3 m) 2 ( 0.10 ´ 10 -3 m)
= 223 ´ 109 N/m2 = 223 GPa (31.3 ´ 106 psi)
6.6 Consider a cylindrical titanium wire 3.0 mm (0.12 in.) in diameter and 2.5 ´ 10 4 mm (1000 in.) long.
Calculate its elongation when a load of 500 N (112 lb f) is applied. Assume that the deformation is totally elastic.
Solution
In order to compute the elongation of the Ti wire when the 500 N load is applied we must employ Equations
6.1, 6.2, and 6.5. Solving for l and realizing that for Ti, E = 107 GPa (15.5 ´ 106 psi) (Table 6.1),
l F
s
Dl = l0e = l0 = 0 =
E
EA0
=
l0F
ö2
æd
Ep ç 0 ÷
è2 ø
=
4l0F
Epd02
(4)(25 m)(500 N)
= 0.0165 m = 16.5 mm (0.65 in.)
(107 ´ 10 9 N/m2 )(p )(3 ´ 10 -3 m) 2
6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the
modulus of elasticity is 115 GPa (16.7 ´ 10 6 psi).
(a) What is the maximum load that may be applied to a specimen with a cross-sectional area of 325 mm2
(0.5 in.2) without plastic deformation?
(b) If the original specimen length is 115 mm (4.5 in.), what is the maximum length to which it may be
stretched without causing plastic deformation?
Solution
(a) This portion of the problem calls for a determination of the maximum load that can be applied without
plastic deformation (F y). Taking the yield strength to be 275 MPa, and employment of Equation 6.1 leads to
F y = s y A0 = (275 ´ 10 6 N/m 2 )(325 ´ 10 -6 m 2 )
= 89,375 N (20,000 lb f)
(b) The maximum length to which the sample may be deformed without plastic deformation is determined
from Equations 6.2 and 6.5 as
æ
sö
li = l0 ç1 + ÷
è
Eø
é
275 MPa ù
= (115 mm) ê1 +
ú = 115.28 mm
115 ´ 10 3 MPa û
ë
(4.51 in.)
6.8 A cylindrical rod of copper (E = 110 GPa, 16 ´ 10 6 psi) having a yield strength of 240 MPa (35,000
psi) is to be subjected to a load of 6660 N (1500 lb f). If the length of the rod is 380 mm (15.0 in.), what must be the
diameter to allow an elongation of 0.50 mm (0.020 in.)?
Solution
This problem asks us to compute the diameter of a cylindrical specimen of copper in order to allow an
elongation of 0.50 mm. Employing Equations 6.1, 6.2, and 6.5, assuming that deformation is entirely elastic
s =
F
=
A0
F
Dl
= E
æd2 ö
l0
pç 0 ÷
ç 4 ÷
è
ø
Or, solving for d 0
d0 =
=
4 l0F
p E Dl
(4) (380 ´ 10 -3 m) (6660 N)
(p) (110 ´ 10 9 N / m2 )(0.50 ´ 10 -3 m)
= 7.65 ´ 10-3 m = 7.65 mm (0.30 in.)
6.9 Compute the elastic moduli for the following metal alloys, whose stress-strain behaviors may be
observed in the “Tensile Tests” module of Virtual Materials Science and Engineering (VMSE): (a) titanium, (b)
tempered steel, (c) aluminum, and (d) carbon steel. How do these values compare with those presented in Table
6.1 for the same metals?
Solution
The elastic modulus is the slope in the linear elastic region (Equation 6.10) as
E =
s - s1
Ds
= 2
De
e2 - e1
Since stress-strain curves for all of the metals/alloys pass through the origin, we make take s1 = 0 and e1 = 0.
Determinations of s2 and e2 are possible by moving the cursor to some arbitrary point in the linear region of the
curve and then reading corresponding values in the “Stress” and “Strain” windows that are located below the plot.
(a) For the titanium alloy, we selected s2 = 404.2 MPa with its corresponding e2 = 0.0038. Therefore,
E =
s 2 - s1
404.2 MPa - 0 MPa
=
= 106, 400 MPa = 106.4 GPa
e2 - e1
0.0038 - 0
The elastic modulus for titanium given in Table 6.1 is 107 GPa, which is in very good agreement with this
value.
(b) For the tempered steel, we selected s2 = 962.2 MPa with its corresponding e2 = 0.0047. Therefore,
E =
s 2 - s1
962.2 MPa - 0 MPa
=
= 204, 700 MPa = 204.7 GPa
e2 - e1
0.0047 - 0
The elastic modulus for steel given in Table 6.1 is 207 GPa, which is in reasonably good agreement with this
value.
(c) For the aluminum, we selected s2 = 145.1 MPa with its corresponding e2 = 0.0021. Therefore,
E =
s 2 - s1
145.1 MPa - 0 MPa
=
= 69,100 MPa = 69.1 GPa
e2 - e1
0.0021 - 0
The elastic modulus for aluminum given in Table 6.1 is 69 GPa, which is in excellent agreement with this
value.
(d) For the carbon steel, we selected s2 = 129 MPa with its corresponding e2 = 0.0006. Therefore,
E =
s 2 - s1
129 MPa - 0 MPa
=
= 215, 000 MPa = 215 GPa
e2 - e1
0.0006 - 0
The elastic modulus for steel given in Table 6.1 is 207 GPa, which is in reasonable agreement with this value.
6.10 Consider a cylindrical specimen of a steel alloy (Figure 6.21) 10.0 mm (0.39 in.) in diameter and 75
mm (3.0 in.) long that is pulled in tension. Determine its elongation when a load of 20,000 N (4,500 lb f) is
applied.
Solution
This problem asks that we calculate the elongation l of a specimen of steel the stress-strain behavior of
which is shown in Figure 6.21. First it becomes necessary to compute the stress when a load of 20,000 N is applied
using Equation 6.1 as
s =
F
=
A0
F
æ d0 ö2
pç ÷
è2ø
=
20, 000 N
æ 10.0 ´ 10 -3 m ö2
pç
÷
2
è
ø
= 255 MPa (37, 700 psi)
Referring to Figure 6.21, at this stress level we are in the elastic region on the stress-strain curve, which corresponds
to a strain of 0.0012. Now, utilization of Equation 6.2 to compute the value of Dl
D l = e l0 = (0.0012)(75mm) = 0.090 mm (0.0036 in.)
6.11 Figure 6.22 shows, for a gray cast iron, the tensile engineering stress–strain curve in the elastic
region. Determine (a) the tangent modulus at 10.3 MPa (1500 psi), and (b) the secant modulus taken to 6.9 MPa
(1000 psi).
Solution
(a) This portion of the problem asks that the tangent modulus be determined for the gray cast iron, the
stress-strain behavior of which is shown in Figure 6.22. In the figure below is shown a tangent draw on the curve at a
stress of 10.3 MPa (1500 psi).
The slope of this line (i.e., s/ e), the tangent modulus, is computed as follows:
Ds
15 MPa - 5 MPa
=
= 1410 MPa = 1.41 GPa (2.04
De
0.0074 - 0.0003
´ 10 5 psi)
(b) The secant modulus taken from the origin is calculated by taking the slope of a secant drawn from the
origin through the stress-strain curve at 6.9 MPa (1,000 psi). This secant is drawn on the curve shown below:
The slope of this line (i.e., s/ e), the secant modulus, is computed as follows:
Ds
15 MPa - 0 MPa
=
= 3190 MPa = 3.19 GPa (4.63
De
0.0047 - 0
´ 10 5 psi)
6.12 As noted in Section 3.15, for single crystals of some substances, the physical properties are
anisotropic; that is, they are dependent on crystallographic direction. One such property is the modulus of
elasticity. For cubic single crystals, the modulus of elasticity in a general [uvw] direction, Euvw, is described by the
relationship
æ
1
1
=
- 3ç
ç
Euvw E 100
è E 100 E 111
1
1
ö
÷ a 2b 2 + b 2 g 2 + g 2a 2
÷
ø
(
)
where E 100 and E 111 are the moduli of elasticity in  and  directions, respectively; α, β, and γ are the
cosines of the angles between [uvw] and the respective , , and  directions. Verify that the Eá110ñ
values for aluminum, copper, and iron in Table 3.3 are correct.
Solution
We are asked, using the equation given in the problem statement, to verify that the modulus of elasticity
values along  directions given in Table 3.3 for aluminum, copper, and iron are correct. The a, b, and g parameters
in the equation correspond, respectively, to the cosines of the angles between the  direction and ,  and
 directions. Since these angles are 45°, 45°, and 90°, the values of a, b, and g are 0.707, 0.707, and 0, respectively.
Thus, the given equation takes the form
1
E<110>
=
æ 1
1 ö
÷÷ (0.707 ) 2 (0.707 ) 2 + (0.707 ) 2 (0) 2 + (0) 2 (0.707 ) 2
- 3çç
E<100>
E
E
è <100>
<111> ø
1
[
æ 1
1 ö
÷÷
- (0.75) çç
E<100>
è E<100> E<111> ø
1
=
Utilizing the values of E
<100>
and E
<111>
1
E<110>
Which leads to, E
<110>
=
from Table 3.3 for Al
é
ù
1
1
1
- (0.75) ê
ú
63.7 GPa
ë 63.7 GPa 76.1 GPa û
= 72.6 GPa, the value cited in the table.
]
For Cu,
1
E<110>
Thus, E
<110>
=
é
ù
1
1
1
- (0.75) ê
ú
66.7 GPa
ë 66.7 GPa 191 .1 GPa û
= 130.3 GPa, which is also the value cited in the table.
Similarly, for Fe
1
E<110>
And E
<110>
=
é
ù
1
1
1
- (0.75) ê
ú
125 .0 GPa
ë 125 .0 GPa 272 .7 GPa û
= 210.5 GPa, which is also the value given in the table.
6.13 In Section 2.6 it was noted that the net bonding energy EN between two isolated positive and
negative ions is a function of interionic distance r as follows:
A B
+
r rn
EN = -
(6.25)
where A, B, and n are constants for the particular ion pair. Equation 6.25 is also valid for the bonding energy
between adjacent ions in solid materials. The modulus of elasticity E is proportional to the slope of the interionic
force–separation curve at the equilibrium interionic separation; that is,
æ dF ö
E µç ÷
è dr ør
o
Derive an expression for the dependence of the modulus of elasticity on these A, B, and n parameters (for the twoion system) using the following procedure:
1. Establish a relationship for the force F as a function of r, realizing that
F=
dEN
dr
2. Now take the derivative dF/dr.
3. Develop an expression for r 0, the equilibrium separation. Since r 0 corresponds to the value of r at the
minimum of the EN-versus-r curve (Figure 2.8b), take the derivative dEN/dr, set it equal to zero, and solve for r,
which corresponds to r 0.
4. Finally, substitute this expression for r 0 into the relationship obtained by taking dF/dr.
Solution
This problem asks that we derive an expression for the dependence of the modulus of elasticity, E, on the
parameters A, B, and n in Equation 6.25. It is first necessary to take dEN/dr in order to obtain an expression for the
force F; this is accomplished as follows:
F =
dE N
dr
=
æ Bö
æ Aö
dç ÷
d ç- ÷
è rø
èr n ø
=
+
dr
dr
A
r2
-
nB
r (n + 1)
The second step is to set this dE /dr expression equal to zero and then solve for r (= r 0). The algebra for this
N
procedu re is carried out in Problem 2.14, with the result that
æ A ö1/(1 - n)
r0 = ç ÷
è nB ø
Next it becomes necessary to take the derivative of the force (dF/dr), which is accomplished as follows:
æ Aö
æ
nB ö
dç ÷
d ç÷
2
(n
dF
èr ø
è r + 1) ø
=
+
dr
dr
dr
=-
2A
r3
+
(n)(n + 1)B
r (n + 2)
Now, substitution of the above expression for r 0 into this equation yields
æ dF ö
2A
(n)(n + 1) B
+
ç ÷ =3/(
1n)
è dr ør
æ Aö
æ A ö(n + 2) /(1- n)
0
ç ÷
ç ÷
è nB ø
è nB ø
which is the expression to which the modulus of elasticity is proportional.
6.14 Using the solution to Problem 6.13, rank the magnitudes of the moduli of elasticity for the following
hypothetical X, Y, and Z materials from the greatest to the least. The appropriate A, B, and n parameters (Equation
IRUW
KHVHW
KUHHP DW
HULDOVDUHW
DEXODW
HG EHORZ W
KH\ \ LHOG ( N in units of electron volts and r in nanometers:
Material
A
B
n
X
2.5
2.0 × 10 –5
Y
2.3
8.0 × 10
–6
Z
3.0
1.5 × 10 –5
8
10.5
9
Solution
This problem asks that we rank the magnitudes of the moduli of elasticity of the three hypothetical metals X,
Y, and Z. From Problem 6.13, it was shown for materials in which the bonding energy is dependent on the interatomic
distance r according to Equation 6.25, that the modulus of elasticity E is proportional to
2A
E µ-
ö3/(1- n)
(n)(n + 1) B
+
æ A ö(n + 2) /(1- n)
ç ÷
è nB ø
æ A
ç ÷
è nB ø
For metal X, A = 2.5, B = 2.0 ´ 10-5, and n = 8. Therefore,
(2)(2.5)
E µ é
ê
ê (8)
ë
ù
2.5
ú
(2 ´ 10 -5 ) úû
3/(1 - 8)
(8)(8 + 1) (2 ´ 10 -5 )
+
é
ù( 8 + 2) /(1 - 8)
2.5
ê
ú
ë (8) (2 ´ 10 -5 ) û
= 1097
For metal Y, A = 2.3, B = 8 ´ 10-6, and n = 10.5. Hence
(2)(2.3)
E µ é
ê
ê (10.5)
ë
2.3
(8 ´
ù 3/(1 - 10.5)
ú
10 -6 úû
)
+
(10.5)(10.5 + 1) (8 ´ 10 -6 )
é
ù(10.5 + 2) /(1 - 10.5)
2.3
ê
ú
ë (10.5) (8 ´ 10 -6 ) û
= 551
And, for metal Z, A = 3.0, B = 1.5 ´ 10-5, and n = 9. Thus
(2)(3.0)
E µ é
ê
ê (9)
ë
ù
3.0
ú
5
(1.5 ´ 10 ) úû
3/(1 - 9)
+
(9)(9 + 1) (1.5 ´ 10 -5 )
é
ù( 9 + 2) /(1 - 9)
3.0
ê
ú
ë (9) (1.5 ´ 10 -5 ) û
= 1024
Therefore, metal X has the highest modulus of elasticity.
Elastic Properties of Materials
6.15 A cylindrical specimen of aluminum having a diameter of 19 mm (0.75 in.) and length of 200 mm (8.0
in.) is deformed elastically in tension with a force of 48,800 N (11,000 lb f). Using the data contained in Table 6.1,
determine the following:
(a) The amount by which this specimen will elongate in the direction of the applied stress.
(b) The change in diameter of the specimen. Will the diameter increase or decrease?
Solution
(a) We are asked, in this portion of the problem, to determine the elongation of a cylindrical specimen of
aluminum. Combining Equations 6.1, 6.2, and 6.5, leads to
s = Ee
F
Dl
=E
æ d2 ö
l0
pç 0 ÷
ç 4 ÷
è ø
Or, solving for Dl (and realizing that E = 69 GPa, Table 6.1), yields
Dl =
=
4F l0
p d02 E
(4)(48, 800 N) (200 ´ 10 -3 m)
= 5 ´ 10 -4 m = 0.50 mm (0.02 in.)
(p) (19 ´ 10 -3 m)2 (69 ´ 10 9 N / m2 )
(b) We are now called upon to determine the change in diameter, Dd . Using Equation 6.8
e
Dd / d0
n = - x = ez
D l / l0
From Table 6.1, for aluminum, n = 0.33. Now, solving the above expression for d yields
Dd = -
n Dl d0
(0.33)(0.50 mm )(19 mm )
= l0
200 mm
= – 1.6 ´ 10-2 mm (– 6.2 ´ 10-4 in.)
The diameter will decrease.
6.16 A cylindrical bar of steel 10 mm (0.4 in.) in diameter is to be deformed elastically by application of a
force along the bar axis. Using the data in Table 6.1, determine the force that will produce an elastic reduction of
3 ´ 10 -3 mm (1.2 ´ 10 -4 in.) in the diameter.
Solution
This problem asks that we calculate the force necessary to produce a reduction in diameter of 3 ´ 10-3 mm
for a cylindrical bar of steel. For a cylindrical specimen, the cross-sectional area is equal to
A0 =
p d02
4
Now, combining Equations 6.1 and 6.5 leads to
F
F
=
= Ee z
A0
pd02
4
s =
And, since from Equation 6.8
ez = -
ex
n
=-
Dd
d0
n
=-
Substitution of this equation into the above expression gives
æ Dd ö
÷÷
= E ççpd02
è nd0 ø
4
F
And, solving for F leads to
d Dd p E
F = - 0
4n
From Table 6.1, for steel, n = 0.30 and E = 207 GPa. Thus,
Dd
nd0
F = -
(10 ´ 10 -3 m)(- 3.0 ´ 10 -6 m) (p) (207
(4)(0.30)
= 16,250 N (3770 lb f)
´ 10 9 N / m2 )
6.17 A cylindrical specimen of some alloy 8 mm (0.31 in.) in diameter is stressed elastically in tension. A
force of 15,700 N (3530 lb f) produces a reduction in specimen diameter of 5 ´ 10 -3 mm (2 ´ 10 -4 in.). Compute
Poisson's ratio for this material if its modulus of elasticity is 140 GPa (20.3 ´ 10 6 psi).
Solution
This problem asks that we compute Poisson's ratio for the metal alloy. From Equations 6.5 and 6.1
ez =
s
F
=
=
E
A0 E
F
ö2
æd
pç 0 ÷ E
è2 ø
=
4F
p d02 E
Since the transverse strain ex is just
ex =
Dd
d0
and Poisson's ratio is defined by Equation 6.8, then
e
Dd / d0
d Dd p E
n = - x = = - 0
æ
ö
ez
4F
ç 4F ÷
ç p d 2E ÷
è 0 ø
= -
(8 ´ 10 -3 m)(-5 ´ 10 -6 m) (p) (140
(4)(15, 700 N)
´ 10 9 N / m 2 )
= 0.280
6.18 A cylindrical specimen of a hypothetical metal alloy is stressed in compression. If its original and
final diameters are 20.000 and 20.025 mm, respectively, and its final length is 74.96 mm, compute its original
length if the deformation is totally elastic. The elastic and shear moduli for this alloy are 105 GPa and 39.7 GPa,
respectively.
Solution
This problem asks that we compute the original length of a cylindrical specimen that is stressed in
compression. It is first convenient to compute the lateral strain ex as
ex =
Dd 20.025 mm - 20.000 mm
=
= 1.25 ´ 10 -3
d0
20.000 mm
In order to determine the longitudinal strain ez ZH QHHG 3RLVVRQV UDW
LR ZKLFK P D\ EHFRP SXW
HG XVLQJ ( TXDW
LRQ
solving for n yields
n =
E
105 ´ 10 3 MPa
-1 =
- 1 = 0.322
2G
(2) (39.7 ´ 10 3 MPa)
Now ez may be computed from Equation 6.8 as
ez = -
ex
1.25 ´ 10 -3
= = - 3.88 ´ 10 -3
n
0.322
Now solving for l0 using Equation 6.2
l0 =
=
li
1 + ez
74.96 mm
= 75.25 mm
1 - 3.88 ´ 10 -3
6.19 Consider a cylindrical specimen of some hypothetical metal alloy that has a diameter of 8.0 mm (0.31
in.). A tensile force of 1000 N (225 lb f) produces an elastic reduction in diameter of 2.8 ´ 10 -4 mm (1.10 ´ 10 -5 in.).
Compute the modulus of elasticity for this alloy, given that Poisson's ratio is 0.30.
Solution
This problem asks that we calculate the modulus of elasticity of a metal that is stressed in tension.
Combining Equations 6.5 and 6.1 leads to
E =
s
F
=
=
ez
A0ez
F
æ d ö2
e zp ç 0 ÷
è2ø
=
4F
e z p d02
From the definition of Poisson's ratio, (Equation 6.8) and realizing that for the transverse strain, ex=
Dd
d0
e
Dd
ez = - x = n
d0 n
Therefore, substitution of this expression for ez into the above equation yields
E =
=
4F
e z p d02
=
4F n
p d0 Dd
(4)(1000 N )(0.30)
= 1.705 ´ 10 11 Pa = 170.5 GPa (24.7
p (8 ´ 10 -3 m)(2.8 ´ 10 -7 m)
´ 10 6 psi)
6.20 A brass alloy is known to have a yield strength of 275 MPa (40,000 psi), a tensile strength of 380
MPa (55,000 psi), and an elastic modulus of 103 GPa (15.0 ´ 10 6 psi). A cylindrical specimen of this alloy 12.7
mm (0.50 in.) in diameter and 250 mm (10.0 in.) long is stressed in tension and found to elongate 7.6 mm (0.30 in.).
On the basis of the information given, is it possible to compute the magnitude of the load that is necessary to
produce this change in length? If so, calculate the load. If not, explain why.
Solution
We are asked to ascertain whether or not it is possible to compute, for brass, the magnitude of the load
necessary to produce an elongation of 7.6 mm (0.30 in.). It is first necessary to compute the strain at yielding from the
yield strength and the elastic modulus, and then the strain experienced by the test specimen. Then, if
e(test) < e(yield)
deformation is elastic, and the load may be computed using Equations 6.1 and 6.5. However, if
e(test) > e(yield)
computation of the load is not possible inasmuch as deformation is plastic and we have neither a stress-strain plot
nor a mathematical expression relating plastic stress and strain. We compute these two strain values as
e(test) =
Dl
7.6 mm
=
= 0.03
l0
250 mm
and
e(yield) =
sy
E
=
275 MPa
= 0.0027
103 ´ 10 3 MPa
Therefore, computation of the load is not possible since e(test) > e(yield).
6.21 A cylindrical metal specimen 12.7 mm (0.5 in.) in d iameter and 250 mm (10 in.) long is to be
VXEM
HFW
HG W
RDW
HQVLOH VW
UHVV RI
0 3D
SVL
DWW
KLVVW
UHVVOHYHOW
KH UHVXOW
LQJ GHIRUP DW
LRQ ZLOOEH W
RW
DOO\
elastic.
(a) If the elongation must be less than 0.080 mm (3.2 ´ 10 -3 in.), which of the metals in Table 6.1 are
suitable candidates? Why?
(b) If, in addition, the maximum permissible diameter decrease is 1.2 ´ 10 -3 mm (4.7 ´ 10 -5 in.) when the
tensile stress of 28 MPa is applied, which of the metals that satisfy the criterion in part (a) are suitable
candidates? Why?
Solution
(a) This part of the problem asks that we ascertain which of the metals in Table 6.1 experience an elongation
of less than 0.080 mm when subjected to a tensile stress of 28 MPa. The maximum strain that may be sustained,
(using Equation 6.2) is just
e =
Dl 0.080 mm
=
= 3.2 ´ 10 -4
l0
250 mm
Since the stress level is given (50 MPa), using Equation 6.5 it is possible to compute the minimum modulus of
elasticity which is required to yield this minimum strain. Hence
E =
s
28 MPa
=
= 87.5 GPa
e
3.2 ´ 10 -4
Which means that those metals with moduli of elasticity greater than this value are acceptable candidates—namely,
brass, Cu, Ni, steel, Ti and W.
(b) This portion of the problem further stipulates that the maximum permissible diameter decrease is 1.2 ´
-3
10 mm when the tensile stress of 28 MPa is applied. This translates into a maximum lateral strain ex(max) as
ex (max) =
Dd
-1.2 ´ 10 -3 mm
=
= - 9.45 ´ 10 -5
d0
12.7 mm
But, since the specimen contracts in this lateral direction, and we are concerned that this strain be less than 9.45 ´ 105 , then the criterion for this part of the problem may be stipulated as - Dd < 9.45 ´ 10 -5.
d0
Now, Poisson’s ratio is defined by Equation 6.8 as
e
n=- x
ez
Dd
For each of the metal alloys let us consider a possible lateral strain, e x =
. Furthermore, since the deformation is
d0
elastic, then, from Equation 6.5, the longitudinal strain, ez is equal to
ez =
s
E
Substituting these expressions for ex and ez into the definition of Poisson’s ratio we have
Dd
e
d
n = - x =- 0
s
ez
E
which leads to the following:
-
Dd n s
=
d0
E
Using values for n and E found in Table 6.1 for the six metal alloys that satisfy the criterion for part (a), and for s = 28
Dd
MPa, we are able to compute a for each alloy as follows:
d0
-
Dd
(0.34)(28 ´ 10 6 N / m2 )
(brass) =
= 9.81 ´ 10 -5
d0
97 ´ 10 9 N / m2
-
Dd
(0.34)(28 ´ 10 6 N / m2 )
(copper) =
= 8.65 ´ 10 -5
d0
110 ´ 10 9 N / m2
-
Dd
(0.34)(28 ´ 10 6 N / m2 )
(titanium) =
= 8.90 ´ 10 -5
d0
107 ´ 10 9 N / m2
-
Dd
(0.31)(28 ´ 10 6 N / m2 )
(nickel) =
= 4.19 ´ 10 -5
d0
207 ´ 10 9 N / m2
-
Dd
(0.30)(28 ´ 10 6 N / m2 )
(steel) =
= 4.06 ´ 10 -5
d0
207 ´ 10 9 N / m2
-
Dd
(0.28)(28 ´ 10 6 N / m2 )
(tungsten) =
= 1.93 ´ 10 -5
d0
407 ´ 10 9 N / m2
Thus, of the above six alloys, only brass will have a negative transverse strain that is greater than 9.45 ´ 10-5 . This
means that the following alloys satisfy the criteria for both parts (a) and (b) of the problem: copper, titanium, nickel,
steel, and tungsten.
6.22 Consider the brass alloy for which the stress-strain behavior is shown in Figure 6.12. A cylindrical
specimen of this material 6 mm (0.24 in.) in diameter and 50 mm (2 in.) long is pulled in tension with a force of
5000 N (1125 lb f). If it is known that this alloy has a Poisson's ratio of 0.30, compute: (a) the specimen
elongation, and (b) the reduction in specimen diameter.
Solution
(a) This portion of the problem asks that we compute the elongation of the brass specimen. The first
calculation necessary is that of the applied stress using Equation 6.1, as
s =
F
=
A0
F
æd ö
pç 0 ÷
è2ø
2
=
5000 N
æ 6 ´ 10 -3 m ö
pç
÷
2
è
ø
2
= 177 ´ 10 6 N/m2 = 177 MPa (25, 000 psi)
From the stress-strain plot in Figure 6.12, this stress corresponds to a strain of about 2.0 ´ 10-3 . From the definition
of strain, Equation 6.2
Dl = e l0 = (2.0 ´ 10 -3) (50 mm) = 0.10 mm
(4 ´ 10 -3 in.)
(b) In order to determine the reduction in diameter d , it is necessary to use Equation 6.8 and the definition
of lateral strain (i.e., e = d/d ) as follows
x
0
Dd = d0ex = - d0 n e z = - (6 mm)(0.30) (2.0 ´ 10 -3)
= – 3.6 ´ 10-3 mm (– 1.4 ´ 10-4 in.)
6.23 A cylindrical rod 100 mm long and having a diameter of 10.0 mm is to be deformed using a tensile
load of 27,500 N. It must not experience either plastic deformation or a diameter reduction of more than 7.5 ´ 10 -3
mm. Of the materials listed as follows, which are possible candidates? Justify your choice(s).
Modulus of Elasticity
(GPa)
Yield Strength
(MPa)
Poisson’s Ratio
70
200
0.33
Brass alloy
101
300
0.34
Steel alloy
207
400
0.30
Titanium alloy
107
650
0.34
Material
Aluminum alloy
Solution
This problem asks that we assess the four alloys relative to the two criteria presented. The first criterion is
that the material not experience plastic deformation when the tensile load of 27,500 N is applied; this means that the
stress corresponding to this load not exceed the yield strength of the material. Upon computing the stress
s =
F
=
A0
F
æd ö
pç 0 ÷
è2ø
2
=
27, 500 N
æ 10 ´ 10 -3 m ö2
pç
÷
2
è
ø
= 350 ´ 10 6 N/m2 = 350 MPa
Of the alloys listed, the Ti and steel alloys have yield strengths greater than 350 MPa.
Relative to the second criterion (i.e., that Dd be less than 7.5 ´ 10-3 mm), it is necessary to calculate the
change in diameter d for these three alloys. From Equation 6.8
Dd
d
E Dd
n = = - 0 =s
ez
s d0
E
ex
Now, solving for d from this expression,
Dd = -
For the steel alloy
n s d0
E
Dd = -
(0.30)(350 MPa ) (10 mm)
= - 5.1 ´ 10 -3 mm
207 ´ 10 3 MPa
Therefore, the steel is a candidate.
For the Ti alloy
Dd = -
(0.34)(350 MPa )(10 mm )
= - 11.1 ´ 10 -3 mm
107 ´ 10 3 MPa
Hence, the titanium alloy is not a candidate.
6.24 A cylindrical rod 380 mm (15.0 in.) long, having a diameter of 10.0 mm (0.40 in.), is to be subjected
to a tensile load. If the rod is to experience neither plastic deformation nor an elongation of more than 0.9 mm
(0.035 in.) when the applied load is 24,500 N (5500 lb f), which of the four metals or alloys listed below are
possible candidates? Justify your choice(s).
Modulus of Elasticity
(GPa)
Yield Strength
(MPa)
Tensile Strength
(MPa)
70
255
420
Brass alloy
100
345
420
Copper
110
250
290
Steel alloy
207
450
550
Material
Aluminum alloy
Solution
This problem asks that we ascertain which of four metal alloys will not (1) experience plastic deformation,
and (2) elongate more than 0.9 mm when a tensile load of 24,500 N is applied. It is first necessary to compute the
VW
UHVV XVLQJ ( TXDW
LRQ
D P DW
HULDOW
R EH Xsed for this application must necessarily have a yield strength greater
than this value. Thus,
s =
F
=
A0
24, 500 N
æ 10.0 ´ 10 -3 m ö2
pç
÷
2
è
ø
= 312 MPa
Of the metal alloys listed, only brass and steel have yield strengths greater than this stress.
Next, we must compute the elongation produced in both brass and steel using Equations 6.2 and 6.5 in order
to determine whether or not this elongation is less than 0.9 mm. For brass
Dl =
s l0
(312 MPa )(380 mm )
=
= 1.19 mm
E
100 ´ 10 3 MPa
Thus, brass is not a candidate. However, for steel
Dl =
s l0
(312 MPa )(380 mm )
=
= 0.57 mm
E
207 ´ 10 3 MPa
Therefore, of these four alloys, only steel satisfies the stipulated criteria.
Tensile Properties
6.25 Figure 6.21 shows the tensile engineering stress–strain behavior for a steel alloy.
(a) What is the modulus of elasticity?
(b) What is the proportional limit?
(c) What is the yield strength at a strain offset of 0.002?
(d) What is the tensile strength?
Solution
Using the stress-strain plot for a steel alloy (Figure 6.21), we are asked to determine several of its mechanical
characteristics.
(a) The elastic modulus is just the slope of the initial linear portion of the curve; or, from the inset and
using Equation 6.10
E =
s 2 - s 1 (200 - 0) MPa
=
= 200 ´ 10 3 MPa = 200 GPa
e2 - e1
(0.0010 - 0)
( 29 ´ 10 6 psi)
The value given in Table 6.1 is 207 GPa.
(b) The proportional limit is the stress level at which linearity of the stress-strain curve ends, which is
approximately 300 MPa (43,500 psi).
(c) The 0.002 strain offset line intersects the stress-strain curve at approximately 400 MPa (58,000 psi).
(d) The tensile strength (the maximum on the curve) is approximately 515 MPa (74,700 psi).
6.26 A cylindrical specimen of a brass alloy having a length of 60 mm (2.36 in.) must elongate only 10.8
mm (0.425 in.) when a tensile load of 50,000 N (11,240 lb f) is applied. Under these circumstances, what must be
the radius of the specimen? Consider this brass alloy to have the stress-strain behavior shown in Figure 6.12.
Solution
We are asked to calculate the radius of a cylindrical brass specimen in order to produce an elongation of
10.8 mm when a load of 50,000 N is applied. It first becomes necessary to compute the strain corresponding to this
elongation using Equation 6.2 as
e =
Dl 10.8 mm
=
= 0.18
l0
60 mm
From Figure 6.12, a stress of 420 MPa (61,000 psi) corresponds to this strain. Since for a cylindrical specimen, stress,
force, and initial radius r 0 are related as
s =
F
p r02
then
r0 =
F
=
ps
50, 000 N
= 0.0062 m = 6.2 mm (0.24 in.)
p (420 ´ 10 6 N / m2 )
6.27 A load of 85,000 N (19,100 lb f) is applied to a cylindrical specimen of a steel alloy (displaying the
stress– strain behavior shown in Figure 6 .21) that has a cross-sectional diameter of 15 mm (0.59 in.).
(a) Will the specimen experience elastic and/or plastic deformation? Why?
(b) If the original specimen length is 250 mm (10 in.), how much will it increase in length when this load
is applied?
Solution
This problem asks us to determine the deformation characteristics of a steel specimen, the stress-strain
behavior for which is shown in Figure 6.21.
(a) In order to ascertain whether the deformation is elastic or plastic, we must first compute the stress, then
locate it on the stress-strain curve, and, finally, note whether this point is on the elastic or plastic region. Thus, from
Equation 6.1
s =
F
=
A0
85, 000 N
æ 15 ´ 10 -3 m ö2
pç
÷
2
è
ø
= 481 ´ 10 6 N/m2 = 481 MPa (69, 900 psi)
The 481 MPa point is beyond the linear portion of the curve, and, therefore, the deformation will be both elastic and
plastic.
(b) This portion of the problem asks us to compute the increase in specimen length. From the stress-strain
curve, the strain at 481 MPa is approximately 0.0135. Thus, from Equation 6.2
Dl = e l0 = (0.0135)(250
mm) = 3.4 mm (0.135 in.)
6.28 A bar of a steel alloy that exhibits the stress-strain behavior shown in Figure 6.21 is subjected to a
W
HQVLOHORDG W
KHVSHFLP HQ LV
PP
LQ ORQJ DQG RI VTXDUHFURVVVHFW
LRQ
PP
LQ RQ D VLGH
(a) Compute the ma gnitude of the load necessary to produce an elongation of 0.45 mm (0.018 in.).
(b) What will be the deformation after the load has been released?
Solution
(a) We are asked to compute the magnitude of the load necessary to produce an elongation of 0.45 mm for
the steel displaying the stress-strain behavior shown in Figure 6.21. First, calculate the strain, and then the
corresponding stress from the plot.
e =
Dl 0.45 mm
=
= 1.5 ´ 10 -3
l0
300 mm
7 KLV LV QHDUW
KHHQG RI W
KHHODVW
LF UHJ LRQ IURP W
KHLQVHWRI ) LJ XUH .21, this corresponds to a stress of about 300 MPa
(43,500 psi). Now, from Equation 6.1
F = sA0 = sb 2
in which b is the cross-section side length. Thus,
F = (300 ´ 10 6 N/m2 ) (4.5 ´ 10 -3 m) 2 = 6075 N
(1366 lb f )
(b) After the load is released there will be no deformation since the material was strained only elastically.
6.29 A cylindrical specimen of aluminum having a diameter of 0.505 in. (12.8 mm) and a gauge length of
2.000 in. (50.800 mm) is pulled in tension. Use the load–elongation characteristics tabulated below to complete
parts (a) through (f).
Length
N
lbf
mm
in.
0
0
50.800
2.000
7,330
1,650
50.851
2.002
15,100
3,400
50.902
2.004
23,100
5,200
50.952
2.006
30,400
6,850
51.003
2.008
34,400
7,750
51.054
2.010
38,400
8,650
51.308
2.020
41,300
9,300
5 1.816
2.040
44,800
10,100
52.832
2.080
46,200
10,400
53.848
2.120
47,300
10,650
54.864
2.160
47,500
10,700
55.880
2.200
46,100
10,400
56.896
2.240
44,800
10,100
57.658
2.270
42,600
9,600
58.420
2.300
36,400
8,200
59.182
2.330
Fracture
(a) Plot the data as engineering stress versus engineering strain.
(b) Compute the modulus of elasticity.
(c) Determine the yield strength at a strain offset of 0.002.
(d) Determine the tensile strength of this alloy.
(e) What is the approximate ductility, in percent elongation?
(f) Compute the modulus of resilience.
Solution
This problem calls for us to make a stress-strain plot for aluminum, given its tensile load-length data, and
then to determine some of its mechanical characteristics.
(a) The data are plotted below on two plots: the first corresponds to the entire stress-strain curve, while for
the second, the curve extends to just beyond the elastic region of deformation.
(b) The elastic modulus is the slope in the linear elastic region (Eq uation 6.10) as
E =
D s 200 MPa - 0 MPa
=
= 62.5 ´ 10 3 MPa = 62.5 GPa (9.1 ´ 10 6 psi)
De
0.0032 - 0
(c) For the yield strength, the 0.002 strain offset line is drawn dashed. It intersects the stress-strain curve at
approximately 285 MPa (41,000 psi ).
(d) The tensile strength is approximately 370 MPa (54,000 psi), corresponding to the maximum stress on the
complete stress-strain plot.
(e) The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by one-hundred. The
W
RW
DOIUDFW
XUH VW
UDLQ DWIUDFW
XUH LV
VXEW
UDFW
LQJ RXWthe elastic strain (which is about 0.005) leaves a plastic strain
of 0.160. Thus, the ductility is about 16%EL.
(f) From Equation 6.14, the modulus of resilience is just
Ur =
s 2y
2E
which, using data computed above gives a value of
Ur =
(285 MPa) 2
= 0.65 MN/m2 = 0.65 ´ 10 6 N/m2 = 6.5 ´ 10 5 J/m3
(2) (62.5 ´ 10 3 MPa)
(93.8
in.- lb f /in.3)
6.30 A specimen of ductile cast iron having a rectangular cross section of dimensions 4.8 mm ´ 15.9 mm
(3/16 in. ´ 5/8 in.) is deformed in tension. Using the load-elongation data tabulated below, complete problems (a)
through (f).
Length
N
lbf
mm
in.
0
0
75.000
2.953
4,740
1,065
75.025
2.954
9,140
2,055
75.050
2.955
12,920
2,900
75.075
2.956
16,540
3,720
75.113
2.957
18,300
4,110
75.150
2.959
20,170
4,530
75.225
2.962
22,900
5,145
75.375
2.968
25,070
5,635
75.525
2.973
26,800
6,025
75.750
2.982
28,640
6,440
76.500
3.012
30,240
6,800
78.000
3.071
31,100
7,000
79.500
3.130
31,280
7,030
81.000
3.189
30,820
6,930
82.500
3.248
29,180
6,560
84.000
3.307
27,190
6,110
85.500
3.366
24,140
5,430
87.000
3.425
18,970
4,265
88.725
3.493
Fracture
(a) Plot the data as engineering stress versus engineering strain.
(b) Compute the modulus of elasticity.
(c) Determine the yield strength at a strain offset of 0.002.
(d) Determine the tensile strength of this alloy.
(e) Compute the modulus of resilience.
(f) What is the ductility, in percent elongation?
Solution
This problem calls for us to make a stress-strain plot for a ductile cast iron, given its tensile load-length data,
and then to determine some of its mechanical characteristics.
(a) The data are plotted below on two plots: the first corresponds to the entire stress-strain curve, while for
the second, the curve extends just beyond the elastic region of deformation.
(b) The elastic modulus is the slope in the linear elastic region (Equation 6.10) as
E =
D s 100 MPa - 0 MPa
=
= 200 ´ 10 3 MPa = 200 GPa
De
0.0005 - 0
(29 ´ 10 6 psi)
(c) For the yield strength, the 0.002 strain offset line is drawn dashed. It intersects the stress-strain curve at
approximately 280 MPa (40,500 psi).
(d) The tensile strength is approximately 410 MPa (59,500 psi), corresponding to the maximum stress on the
complete stress-strain plot.
(e) From Equation 6.14, the modulus of resilience is just
Ur =
s 2y
2E
which, using data computed above, yields a value of
Ur =
(280 ´ 10 6 N / m2 ) 2
(2) (200 ´ 10 9 N / m2 )
= 1.96 ´ 10 5 J/m3
(28.3 in. - lb f /in.3)
(f) The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by one-hundred. The
W
RW
DOIUDFW
XUH VW
UDLQ DWIUDFW
XUH LV
VXEW
UDFW
LQJ RXWW
KHHODVW
LF VW
UDLQ ZKLFK LVDERXW
of 0.184. Thus, the ductility is about 18.4%EL.
OHDYHVDSODVW
LF VW
rain
6.31 For the titanium alloy, whose stress strain behavior may be observed in the “Tensile Tests” module of
Virtual Materials Science and Engineering (VMSE), determine the following:
(a) the approximate yield strength (0.002 strain offset),
(b) the tensile strength, and
(c) the approximate ductility, in percent elongation.
How do these values compare with those for the two Ti-6Al-4V alloys presented in Table B.4 of Appendix B?
Solution
(a) It is possible to do a screen capture and then print out the entire stress-strain curve for the Ti alloy. The
intersection of a straight line parallel to the initial linear region of the curve and offset at a strain of 0.002 with this
curve is at approximately 720 MPa.
(b) The maximum reading in the stress window located below the plot as the curser point is dragged along
the stress-strain curve is 1000 MPa, the value of the tensile strength.
(c) The approximate percent elongation corresponds to the strain at fracture multiplied by 100 (i.e., 12%)
minus the maximum elastic strain (i.e., value of strain at which the linearity of the curve ends multiplied by 100—in
W
KLVFDVHDERXW
W
KLVJ LYHVDYDOXHRI DERXW
(/
From Table B.4 in Appendix B, yield strength, tensile strength, and percent elongation values for the anneal
Ti-6Al-4V are 830 MPa, 900 MPa, and 14%EL, while for the solution heat treated and aged alloy, the corresponding
values are 1103 MPa, 1172 MPa, and 10%EL. Thus, tensile strength and percent elongation values for the VMSE
alloy are slightly lower than for the annealed material in Table B.4 (720 vs 830 MPa, and 11.5 vs. 14 %EL), whereas the
tensile strength is slightly higher (1000 vs. 900 MPa).
6.32 For the tempered steel alloy, whose stress strain behavior may be observed in the “Tensile Tests”
module of Virtual Materials Science and Engineering (VMSE), determine the following:
(a) the approximate yield strength (0.002 strain offset),
(b) the tensile strength, and
(c) the approximate ductility, in percent elongation.
How do these values compare with those for the oil-quenched and tempered 4140 and 4340 steel alloys presented
in Table B.4 of Appendix B?
Solution
(a) It is possible to do a screen capture and then print out the entire stress-strain curve for the tempered
steel alloy. The intersection of a straight line parallel to the initial linear region of the curve and offset at a strain of
0.002 with this curve is at approximately 1430 MPa.
(b) The maximum reading in the stress window located below the plot as the curser point is dragged along
the stress-strain curve is 1656 MPa, the value of the tensile strength.
(c) The approximate percent elongation corresponds to the strain at fracture multiplied by 100 (i.e., 14.8%)
minus the maximum elastic strain (i.e., value of strain at which the linearity of the curve ends multiplied by 100—in
W
KLVFDVHDERXW
W
KLVJ LYHVDYDOXHRI DERXW
(/
For the oil-quenched and tempered 4140 and 4340 steel alloys, yield strength values presented in Table B.4
RI \$ SSHQGL[ % DUH
0 3D DQG
0 3D UHVSHFW
LYHO\ W
KHVH YDOXHV DUH VRP HZKDWODUJ HUW
KDQ W
KH
0 3DIRU
the tempered steel alloy of VMSE. Tensile strength values for these 4140 and 4340 alloys are, respectively 1720 MPa
and 1760 MPa (compared to 1656 MPa for the VMSE steel). And, finally, the respective ductilities for the 4140 and
4340 alloys are 11.5%EL and 12%EL, which are slightly lower than the 14%EL value for the VMSE steel.
6.33 For the aluminum alloy, whose stress strain behavior may be observed in the “Tensile Tests” module
of Virtual Materials Science and Engineering (VMSE), determine the following:
(a) the approximate yield strength (0.002 strain offset),
(b) the tensile strength, and
(c) the approximate ductility, in percent elongation.
How do these values compare with those for the 2024 aluminum alloy (T351 temper) presented in Table B.4 of
Appendix B?
Solution
(a) It is possible to do a screen capture and then print out the entire stress-strain curve for the aluminum
alloy. The intersection of a straight line parallel to the initial linear region of the curve and offset at a strain of 0.002
with this curve is at approximately 300 MPa.
(b) The maximum reading in the stress window located below the plot as the curser point is dragged along
the stress-strain curve is 484 MPa, the value of the tensile strength.
(c) The approximate percent elongation corresponds to the strain at fracture multiplied by 100 (i.e., 22.4%)
minus the maximum elas tic strain (i.e., value of strain at which the linearity of the curve ends multiplied by 100—in
W
KLVFDVHDERXW
W
KLVJ LYHVDYDOXHRI DERXW
(/
For the 2024 aluminum alloy (T351 temper), the yield strength value presented in Table B.4 of Appendix B is
325, which is slightly larger than the 300 MPa for the aluminum alloy of VMSE. The tensile strength value for the
2024-T351 is 470 MPa (compared to 484 MPa for the VMSE alloy). And, finally, the ductility for 2024-T351 is 20%EL,
which is about the same as for the VMSE aluminum (21.9%EL).
6.34 For the (plain) carbon steel alloy, whose stress strain behavior may be observed in the “Tensile
Tests” module of Virtual Materials Science and Engineering (VMSE), determine the following:
(a) the approximate yield strength,
(b) the tensile strength, and
(c) the approximate ductility, in percent elongation.
Solution
(a) It is possible to do a screen capture and then print out the entire stress-strain curve for the plain carbon
steel alloy. Inasmuch as the stress-strain curve displays the yield point phenomenon, we take the yield strength as
the lower yield point, which, for this steel, is about 225 MPa.
(b) The maximum reading in the stress window located below the plot as the curser point is dragged along
the stress-strain curve is 274 MPa, the value of the tensile strength.
(c) The approximate percent elongation corresponds to the strain at fracture multiplied by 100 (i.e., 43.0%)
minus the maximum elastic strain (i.e., value of strain at which the linearity of the curve ends multiplied by 100—in
W
KLVFDVHDERXW
W
KLVJ LYHVDYDOXHRI DERXW
(/
6.35 A cylindrical metal specimen having an original diameter of 12.8 mm (0.505 in.) and gauge length of
50.80 mm (2.000 in.) is pulled in tension until fracture occurs. The diameter at the point of fracture is 6.60 mm
(0.260 in.), and the fractured gauge length is 72.14 mm (2.840 in.). Calculate the ductility in terms of percent
reduction in area and percent elongation.
Solution
This problem calls for the computation of ductility in both percent reduction in area and percent elongation.
Percent reduction in area is computed using Equation 6.12 as
ædf
æ d ö2
pç 0 ÷ - pç
è2ø
è 2
%RA =
2
æd ö
pç 0 ÷
è2ø
ö2
÷
ø
´ 100
in which d 0 and d f are, respectively, the original and fracture cross-sectional areas. Thus,
æ 12.8 mm ö2
æ 6.60 mm
pç
÷ - pç
è
ø
è
2
2
%RA =
2
æ 12.8 mm ö
pç
÷
è
ø
2
ö2
÷
ø
´ 100 = 73.4%
While, for percent elongation, we use Equation 6.11 as
æ l f - l0 ö
%EL = ç
÷ ´ 100
è l0 ø
=
72.14 mm - 50.80 mm
´ 100 = 42%
50.80 mm
6.36 Calculate the moduli of resilience for the materials having the stress–strain behaviors shown in
Figures 6.12 and 6.21.
Solution
This problem asks us to calculate the moduli of resilience for the materials having the stress-strain behaviors
shown in Figures 6.12 and 6.21. According to Equation 6.14, the modulus of resilience Ur is a function of the yield
strength and the modulus of elasticity as
Ur =
s 2y
2E
The values for s and E for the brass in Figure 6.12 are determined in Example Problem 6.3 as 250 MPa (36,000 psi) and
y
93.8 GPa (13.6 ´ 106 psi), respectively. Thus
Ur =
(250 MPa ) 2
= 3.32 ´ 10 5 J/m3
(2) (93.8 ´ 10 3 MPa)
(48.2 in. - lb f /in.3)
Values of the corresponding parameters for the steel alloy (Figure 6.21) are d etermined in Problem 6.25 as 400
MPa (58,000 psi) and 200 GPa (29 ´ 106 psi), respectively, and therefore
Ur =
( 400 MPa ) 2
200 ´ 10 3 MPa
(2) (
)
= 4.0 ´ 10 5 J/m3
(58
in.- lb f /in.3)
6.37 Determine the modulus of resilience for each of the following alloys:
Yield Strength
Material
MPa
psi
Steel alloy
550
80,000
Brass alloy
350
50,750
Aluminum alloy
250
36,250
Titanium alloy
800
116,000
Use modulus of elasticity values in Table 6.1.
Solution
The moduli of resilience of the alloys listed in the table may be determined using Equation 6.14. Yield
strength values are provided in this table, whereas the elastic moduli are tabulated in Table 6.1.
For steel
Ur =
=
(550 ´ 10 6 N / m2 ) 2
(2) (207 ´ 10 9 N / m2 )
s 2y
2E
= 7.31 ´ 10 5 J/m3
(107
in.- lb f /in.3)
For the brass
Ur =
(350 ´ 10 6 N / m2 ) 2
(2) (97 ´ 10 9 N / m2 )
= 6.31 ´ 10 5 J/m3
(92.0
in.- lb f /in.3)
For the aluminum alloy
Ur =
(250 ´ 10 6 N / m2 ) 2
(2) (69 ´ 10 9 N / m2 )
= 4.53 ´ 10 5 J/m3 (65.7 in.- lb f /in.3 )
And, for the titanium alloy
Ur =
(800 ´ 10 6 N / m2 ) 2
(2) (107 ´ 10 9 N / m2 )
= 30.0 ´ 10 5 J/m3
(434
in.- lb f /in.3)
6.38 A brass alloy to be used for a spring application must have a modulus of resilience of at least 0.75
MPa (110 psi). What must be its minimum yield strength?
Solution
The modulus of resilience, yield strength, and elastic modulus of elasticity are related to one another
W
KURXJ K ( TXDW
LRQ
W
KH YDOXH RI E for brass given in Table 6.1 is 97 GPa. Solving for sy from this expression
yields
sy =
2U r E =
(2) (0.75 MPa) (97 ´ 103 MPa)
= 381 MPa (55,500 psi)
True Stress and Strain
6.39 Show that Equations 6.18a and 6.18b are valid when there is no volume change during deformation.
Solution
To show that Equation 6.18a is valid, we must first rearrange Equation 6.17 as
Ai =
A0 l0
li
Substituting this expression into Equation 6.15 yields
sT =
æl ö
F
F æ li ö
=
ç ÷ = sç i ÷
Ai
A0 è l0 ø
è l0 ø
But, from Equation 6.2
l
e = i - 1
l0
Or
li
l0
= e + 1
Thus,
æl ö
sT = sçç i ÷÷ = s (e + 1)
è l0 ø
For Equation 6.18b
eT = ln (1 + e)
is valid since, from Equation 6.16
æl ö
eT = ln ç i ÷
è l0 ø
and
li
l0
from above.
=e + 1
6.40 Demonstrate that Equation 6.16, the expression defining true strain, may also be represented by
T
æA ö
= ln ç 0 ÷
è Ai ø
when specimen volume remains constant during deformation. Which of these two expressions is more valid during
necking? Why?
Solution
This problem asks us to demonstrate that true strain may also be represented by
T
æA ö
= ln ç 0 ÷
è Ai ø
Rearrangement of Equation 6.17 leads to
li
l0
=
A0
Ai
Thus, Equation 6.16 takes the form
T
The expression
T
æl ö
æA ö
= ln ç i ÷ = ln ç 0 ÷
è l0 ø
è Ai ø
æA ö
= ln ç 0 ÷ is more valid during necking because Ai is taken as the area of the neck.
è Ai ø
6.41 Using the data in Problem 6.28 and Equations 6.15, 6.16, and 6.18a, generate a true stress–true
VW
UDLQ SORWIRU DOXP LQXP ( TXDW
LRQ
D EHFRP HV LQYDOLG SDVWW
KH SRLQWDWZKLFK QHFNLQJ EHJ LQV W
KHUHIRUH
measured diameters are given below for the last four data points, which should be used in true stress computations.
Length
Diameter
N
lbf
mm
in.
mm
in.
46,100
10,400
56.896
2.240
11.71
0.461
42,400
10,100
57.658
2.270
10.95
0.431
42,600
9,600
58.420
2.300
10.62
0.418
36,400
8,200
59.182
2.330
9.40
0.370
Solution
These true stress-strain data are plotted below.
6.42 A tensile test is performed on a metal specimen, and it is found that a true plastic strain of 0.20 is
SURGXFHG ZKHQ D W
UXH VW
UHVVRI
0 3D
SVL LVDSSOLHG IRUW
KH VDP H P HW
DO W
KH YDOXH RI . LQ ( TXDW
LRQ
6.19 is 860 MPa (125,000 psi). Calculate the true strain that results from the application of a true stress of 600
MPa (87,000 psi).
Solution
It first becomes necessary to solve for n in Equation 6.19. Taking logarithms of this expression and after
rearrangement we have
n =
log sT - log K
log eT
And, incorporating values of the parameters provided in the problem statement leads to
n=
log (575 MPa ) - log (860 MPa )
= 0.250
log (0.20)
Expressing eT as the dependent variable (Equation 6.19), and then solving for its value from the data stipulated in the
problem statement, leads to
æ s ö1/n æ 600 MPa ö1/0.250
eT = ç T ÷ = ç
= 0.237
÷
èK ø
è 860 MPa ø
6.43 For some metal alloy, a true stress of 415 MPa (60,175 psi) produces a plastic true strain of 0.475.
How much will a specimen of this material elongate when a true stress of 325 MPa (46,125 psi) is applied if the
original length is 300 mm (11.8 in.)? Assume a value of 0.25 for the strain-hardening exponent n.
Solution
Solution of this problem requires that we utilize Equation 6.19. It is first necessary to solve for K from the
given true stress and strain. Rearrangement of this equation yields
K =
sT
415 MPa
=
= 500 MPa (72, 500 psi)
n
(eT )
(0.475 ) 0.25
Next we must solve for the true strain produced when a true stress of 325 MPa is applied, also using Equation 6.19.
Thus
æl ö
æ s ö1/n æ 325 MPa ö1/0.25
eT = ç T ÷ = ç
= 0.179 = ln ç i ÷
÷
èK ø
è 500 MPa ø
è l0 ø
Now, solving for li gives
li = l0 e 0.179 = (300 mm) e 0.179 = 358.8 mm (14.11 in.)
And finally, the elongation l is just
Dl = li - l0 = 358.8 mm - 300 mm = 58.8 mm (2.31 in.)
6.44 The following true stresses produce the corresponding true plastic strains for a brass alloy:
True Stress (psi)
True Strain
50,000
0.10
60,000
0.20
What true stress is necessary to produce a true plastic strain of 0.25?
Solution
For this problem, we are given two values of eT and sT, from which we are asked to calculate the true stress
which produces a true plastic strain of 0.25. Employing Equation 6.19, we may set up two simultaneous equations
with two unknowns (the unknowns being K and n), as
log (50,000 psi) = log K + n log (0.10)
log (60,000 psi) = log K + n log (0.20)
Solving for n from these two expressions yields
n=
log (50, 000) - log (60, 000)
= 0.263
log (0.10 ) - log (0.20)
and for K
log K = 4.96 or K = 104.96 = 91,623 psi
Thus, for eT = 0.25
s T = K (eT ) n = (91, 623 psi)(0.25) 0.263 = 63, 700 psi (440 MPa)
6.45 For a brass alloy, the following engineering stresses produce the corresponding plastic engineering
strains, prior to necking:
Engineering Stress (MPa)
Engineering Strain
235
0.194
250
0.296
On the basis of this information, compute the engineering stress necessary to produce an engineering strain of 0.25.
Solution
For this problem we first need to convert engineering stresses and strains to true stresses and strains so
that the constants K and n in Equation 6.19 may be determined. Since sT = s(1 + e) then
s T 1 = (235 MPa)(1+ 0.194) = 280 MPa
s T 2 = (250 MPa)(1+ 0.296) = 324 MPa
Similarly for strains, since eT = ln(1 + e) then
eT 1 = ln (1 + 0.194) = 0.177
eT 2 = ln (1 + 0.296) = 0.259
Taking logarithms of Equation 6.19, we get
log sT = log K + n log eT
which allows us to set up two simultaneous equations for the above pairs of true stresses and true strains, with K
and n as unknowns. Thus
log (280) = log K + n log (0.177)
log (324) = log K + n log (0.259)
Solving for these two expressions yields K = 543 MPa and n = 0.383.
Now, converting e = 0.25 to true strain
eT = ln (1 + 0.25) = 0.223
The corresponding sT to give this value of eT (using Equation 6.19) is just
s T = KeTn = (543 MPa)(0.223) 0.383 = 306 MPa
Now converting this value of sT to an engineering stress using Equation 6.18a gives
s =
sT
306 MPa
=
= 245 MPa
1 + e 1 + 0.25
6.46 Find the toughness (or energy to cause fracture) for a metal that experiences both elastic and plastic
deformation. Assume Equation 6.5 for elastic deformation, that the modulus of elasticity is 172 GPa (25 ´ 10 6 psi),
and that elastic deforma tion terminates at a strain of 0.01. For plastic deformation, assume that the relationship
between stress and strain is described by Equation 6.19, in which the values for K and n are 6900 MPa (1 ´ 10 6
psi) and 0.30, respectively. Furthermore, plastic deformation occurs between strain values of 0.01 and 0.75, at
which point fracture occurs.
Solution
This problem calls for us to compute the toughness (or energy to cause fracture). The easiest way to do
this is to integrate both elastic and plastic regions, and then add them together.
Toughness = ò s de
0.01
=
ò
0
Ee2
=
2
=
0.01
0
0.75
Ee d e +
ò Ken d e
0.01
K
+
e(n+ 1)
(n + 1)
0.75
0.01
172 ´ 10 9 N/m2
6900 ´ 10 6 N/ m2
(0.01) 2 +
(0.75)1.3 - (0.01) 1.3
2
(1.0 + 0.3)
[
= 3.65 ´ 109 J/m3 (5.29 ´ 105 in.-lb /in.3 )
f
]
6.47 For a tensile test, it can be demonstrated that necking begins when
ds T
= sT
deT
(6.26)
Using Equation 6.19, determine the value of the true strain at this onset of necking.
Solution
Let us take the derivative of Equation 6.19, set it equal to sT, and then solve for eT from the resulting
expression. Thus
[
]
d K (eT ) n
= Kn(eT )(n- 1) = sT
d eT
n
However, from Equation 6.19, s = K(e ) , which, when substituted into the above expression, yields
T
T
Kn(eT )(n - 1) = K (eT ) n
Now solving for eT from this equation leads to
e =n
T
as the value of the true strain at the onset of necking.
6.48 Taking the logarithm of both sides of Equation 6.19 yields
log σT = log K + n log
Thus, a plot of log σT versus log
T
(6.27)
T
in the plastic region to the point of necking should yield a straight line having
a slope of n and an intercept (at log σT = 0) of log K.
Using the appropriate data tabulated in Problem 6.29, make a plot of log σT versus log
T
and determine
the values of n and K. It will be necessary to convert engineering stresses and strains to true stresses and strains
usin g Equations 6.18a and 6.18b.
Solution
This problem calls for us to utilize the appropriate data from Problem 6.29 in order to determine the values of
n and K for this material. From Equation 6.27 the slope and intercept of a log sT versus log eT plot will yield n and log
K UHVSHFW
LYHO\
+ RZHYHU ( TXDW
LRQ
LV RQO\ YDOLG LQ W
KH UHJ LRQ RI SODVW
LF GHIRUP DW
LRQ W
RW
KH SRLQWRI QHFNLQJ
thus, only the 7th, 8th, 9th, and 10th data points may be utilized. The log-log plot with these data points is given
below.
The slope yields a value of 0.136 for n , whereas the intercept gives a value of 2.7497 for log K, and thus K = 102.7497
= 562 MPa.
Elastic Recovery After Plastic Deformation
6.49 A cylindrical specimen of a brass alloy 7.5 mm (0.30 in.) in diameter and 90.0 mm (3.54 in.) long is
pulled in tension with a force of 6000 N (1350 lb f); the force is subsequently released.
(a) Compute the final length of the specimen at this time. The tensile stress–strain behavior for this alloy
is shown in Fig ure 6.12.
(b) Compute the final specimen length when the load is increased to 16,500 N (3700 lb f) and then
released.
Solution
(a) In order to determine the final length of the brass specimen when the load is released, it first becomes
necessary to co P SXW
HW
KHDSSOLHG VW
UHVVXVLQJ ( TXDW
LRQ
s =
F
=
A0
F
æd ö
pç 0 ÷
è2ø
2
=
W
KXV
6000 N
æ 7.5 ´ 10 -3 m ö2
pç
÷
2
è
ø
Upon locating this point on the stress-VW
UDLQ FXUYH ) LJ XUH
= 136 MPa (19, 000 psi)
ZH QRW
HW
KDWLWLV LQ W
KH OLQHDU HODVW
LF UHJ LRQ
therefore, when the load is released the specimen will return to its original length of 90 mm (3.54 in.).
(b) In this portion of the problem we are asked to calculate the final length, after load release, when the load
is increased to 16,500 N (3700 lb f). Again, computing the stress
s =
16, 500 N
æ 7.5 ´ 10 -3 m ö2
pç
÷
2
è
ø
= 373 MPa (52, 300 psi)
The point on the stress-strain curve corresponding to this stress is in the plastic region. We are able to estimate the
amount of permanent strain by drawing a straight line parallel to the linear elastic region; this line intersects the
strain axis at a strain of about 0.08 which is the amount of plastic strain. The final specimen length li may be
determined from a rearranged form of Equation 6.2 as
li = l0(1 + e) = (90 mm)(1 + 0.08) = 97.20 mm (3.82 in.)
6.50 A steel alloy specimen having a rectangular cross section of dimensions 12.7 mm × 6.4 mm (0.5 in. ×
0.25 in.) has the stress– strain behavior shown in Figure 6.21. If this specimen is subjected to a tensile force of
38,000 N (8540 lb f) then
(a) Determine the elastic and plastic strain values.
(b) If its original length is 460 mm (18.0 in.), what will be its final length after the load in part (a) is
applied and then released?
Solution
(a) We are asked to determine both the elastic and plastic strain values when a tensile force of 38,000 N
(8540 lb f) is applied to the steel specimen and then released. First it becomes necessary to determine the applied
VW
UHVVXVLQJ ( TXDW
LRQ
W
KXV
s =
F
F
=
A0
b0 d0
where b 0 and d 0 are cross-sectional width and depth (12.7 mm and 6.4 mm, respectively). Thus
s =
(12.7
38, 000 N
= 468 ´ 10 6 N / m2 = 468 MPa (68, 300 psi)
´ 10 -3 m)(6.4 ´ 10 -3 m)
From Figure 6.21, this point is in the plastic region so the specimen will be both elastic and plastic strains. The total
strain at this point, et, is about 0.010. We are able to estimate the amount of permanent strain recovery ee from
Hooke's law, Equation 6.5 as
ee =
s
E
And, since E = 207 GPa for steel (Table 6.1)
ee =
468 MPa
= 0.00226
207 ´ 10 3 MPa
The value of the plastic strain, ep is just the difference between the total and elastic strains; that is
ep = et – ee = 0.010 – 0.00226 = 0.00774
(b) If the initial length is 460 mm (18.0 in.) then the final specimen length li may be determined from a
rearranged form of Equation 6.2 using the plastic strain value as
li = l0(1 + ep) = (460 mm)(1 + 0.00774) = 463.6 mm (18.14 in.)
Hardness
6.51 (a) A 10-mm-diameter Brinell hardness indenter produced an indentation 1.62 mm in diameter in a
steel alloy when a load of 500 kg was used. Compute the HB of this material.
(b) What will be the diameter of an indentation to yield a hardness of 450 HB when a 500 kg load is
used?
Solution
(a) We are asked to compute the Brinell hardness for the given indentation. It is necessary to use the
equation in Table 6.5 for HB, where P = 500 kg, d = 1.62 mm, and D = 10 mm. Thus, the Brinell hardness is computed
as
2P
HB =
[
pD D -
=
D2 - d2
]
(2)(500 kg )
[
(p)(10 mm) 10 mm -
(10 mm) 2 - (1.62 mm) 2
]
= 241
(b) This part of the problem calls for us to determine the indentation diameter d wh ich will yield a 450 HB
when P = 500 kg. Solving for d from the equation in Table 6.5 gives
d=
=
2
é
2P ù
D 2 - êD ú
(HB)p D û
ë
2
é
(2)(500 kg) ù
(10mm) 2 - ê10 mm ú = 1.19 mm
(450)(p)(10 mm) û
ë
6.52 Estimate the Brinell and Rockwell hardnesses for the following:
(a) The naval brass for which the stress– strain behavior is shown in Figure 6.12.
(b) The steel alloy for which the stress– strain behavior is shown in Figure 6.21.
Solution
This problem calls for estimations of Brinell and Rockwell hardnesses.
(a) For the brass specimen, the stress-strain behavior for which is shown in Figure 6.12, the tensile strength
is 450 MPa (65,000 psi). From Figure 6.19, the hardness for brass corresponding to this tensile strength is about 125
HB or 70 HRB.
(b) The steel alloy (Figure 6.21) has a tensile strength of about 515 MPa (74,700 psi) [Problem 6.25(d)]. This
corresponds to a hardness of about 160 HB or ~90 HRB from the line for steels in Figure 6.19. Alternately, using
Equation 6.20a
HB =
TS(MPa) 515 MPa
=
= 149
3.45
3.45
6.53 Using the data represented in Figure 6.19, specify equations relating tensile strength and Brinell
hardness for brass and nodular cast iron, similar to Equations 6.20a and 6.20b for steels.
Solution
These equations, for a straight line, are of the form
TS = C + (E)(HB)
where TS is the tensile strength, HB is the Brinell hardness, and C and E are constants, which need to be determined.
One way to solve for C and E is analytically--establishing two equations using TS and HB data points on
the plot, as
(TS)1 = C + (E)(BH)1
(TS)2 = C + (E)(BH)2
Solving for E from these two expressions yields
E =
(TS)1 - (TS) 2
(HB) 2 - (HB)1
For nodular cast iron, if we make the arbitrary choice of (HB)1 and (HB)2 as 200 and 300, respectively, then, from
Figure 6.19, (TS)1 and (TS)2 take on values of 600 MPa (87,000 psi) and 1100 MPa (160,000 psi), respectively.
Substituting these values into the above expression and solving for E gives
E =
600 MPa - 1100 MPa
= 5.0 MPa/HB (730 psi/HB)
200 HB - 300 HB
Now, solving for C yields
C = (TS)1 – (E)(BH)1
= 600 MPa - (5.0 MPa/HB)(200 HB) = – 400 MPa (– 59,000 psi)
Thus, for nodular cast iron, these two equations take the form
TS(MPa) = – 400 + 5.0 x HB
TS(psi) = – 59,000 + 730 x HB
Now for brass, we take (HB)1 and (HB)2 as 100 and 200, respectively, then, from Figure 7.31, (TS)1 and (TS)2
take on values of 370 MPa (54,000 psi) and 660 MPa (95,000 psi), respectively. Substituting these values into the
above expression and solving for E gives
E =
370 MPa - 660 MPa
= 2.9 MPa/HB (410 psi/HB)
100 HB - 200 HB
Now, solving for C yields
C = (TS)1 – (E)(BH)1
= 370 MPa – (2.9 MPa/HB)(100 HB) = 80 MPa (13,000 psi)
Thus, for brass these two equations take the form
TS(MPa) = 80 + 2.9 x HB
TS(psi) = 13,000 + 410 x HB
Variability of Material Properties
6.54 Cite five factors that lead to scatter in measured material properties.
Solution
The five IDFW
RUV W
KDWOHDG W
R VFDW
W
HULQ P HDVXUHG P DW
HULDOSURSHUW
LHV DUH W
KH IROORZLQJ
YDULDW
LRQ LQ VSHFLP HQ IDEULFDW
LRQ SURFHGXUH
inhomogeneities and/or compositional differences.
RSHUDW
RU ELDV
DSSDUDW
XV FDOLEUDW
LRQ
W
HVWP HW
KRG
DQG
P DW
HULDO
6.55 Below are tabulated a number of Rockwell B hardness values that were measured on a single steel
specimen. Compute average and standard deviation hardness values.
83.3
80.7
86.4
88.3
84.7
85.2
82.8
87.8
86.9
86.2
83.5
84.4
87.2
85.5
86 .3
Solution
The average of the given hardness values is calculated using Equation 6.21 as
15
å HRBi
HRB =
=
i=1
15
83.3 + 88.3 + 82.8 . . . . + 86.3
= 85.3
15
And we compute the standard deviation using Equation 6.22 as follows:
15
2
å (HRBi - HRB)
i=1
s =
15 - 1
é (83.3 - 85.3) 2 + (88.3 - 85.3) 2 + . . . . + (86.3 - 85.3) 2 ù1/2
=ê
ú
14
ë
û
=
60.31
= 2.08
14
Design/Safety Factors
6.56 Upon what three criteria are factors of safety based?
Solution
The criteria upon which factors of safety are based are (1) consequences of failure, (2) previous experience,
(3) accuracy of measurement of mechanical forces and/or material properties, and (4) economics.
6.57 Determine working stresses for the two alloys that have the stress–strain behaviors shown in Figures
6.12 and 6.21.
Solution
The working stresses for the two alloys the stress-strain behaviors of which are shown in Figures 6.12 and
6.21 are calculated by dividing the yield strength by a factor of safety, which we will take to be 2. For the brass alloy
(Figure 6.12), since sy = 250 MPa (36,000 psi), the working stress is 125 MPa (18,000 psi), whereas for the steel alloy
(Figure 6.21), sy = 400 MPa (58,000 psi), and, therefore, sw = 200 MPa (29,000 psi).
DESIGN PROBLEMS
6.D1 A large tower is to be supported by a series of steel wires. It is estimated that the load on each wire
will be 11,100 N (2500 lb f). Determine the minimum required wire diameter assuming a factor of safety of 2 and a
yield strength of 1030 MPa (150,000 psi).
Solution
For this problem the working stress is computed using Equation 6.24 with N = 2, as
sw =
sy
2
=
1030 MPa
= 515 MPa (75, 000 psi )
2
Since the force is given, the area may be determined from Equation 6.1, and subsequently the original diameter d 0
may be calculated as
A0 =
æ d ö2
F
= pç 0 ÷
sw
è 2 ø
And
d0 =
4F
=
p sw
(4)(11,100 N)
p (515 ´ 10 6 N / m2 )
= 5.23 ´ 10-3 m = 5.23 mm (0.206 in.)
6.D2 (a) Gaseous hydrogen at a constant pressure of 1.013 MPa (10 atm) is to flow within the inside of a
thin-walled cylindrical tube of nickel that has a radius of 0.1 m. The temperature of the tube is to be 300°C and
the pressure of hyd rogen outside of the tube will be maintained at 0.01013 MPa (0.1 atm). Calculate the minimum
wall thickness if the diffusion flux is to be no greater than 1 ´ 10 -7 mol/m2-s. The concentration of hydrogen in the
nickel, CH (in moles hydrogen per m3 of Ni) is a function of hydrogen pressure, P H2 (in MPa) and absolute
temperature (T) according to
æ 12.3 kJ/mol ö
CH = 30.8 pH 2 expç÷
è
ø
RT
(6.28)
Furthermore, the diffusion coefficient for the diffusion of H in Ni depends on temperature as
æ 39.56 kJ/mol ö
DH = 4.76 ´ 10 -7 expç÷
è
ø
RT
(6.29)
(b) For thin-walled cylindrical tubes that are pressurized, the circumferential stress is a function of the
pressure difference across the wall (∆p), cylinder radius (r), and tube thickness (∆x) as
s =
r Dp
4 Dx
(6.30)
Compute the circumferential stress to which the walls of this pressurized cylinder are exposed.
(c) The room-temperature yield strength of Ni is 100 MPa (15,000 psi) and, furthermore, sy diminishes
about 5 MPa for every 50°C rise in temperature. Would you expect the wall thickness computed in part (b) to be
suitable for this Ni cylinder at 300°C? Why or why not?
(d) If this thickness is found to be suitable, compute the minimum thickness that could be used without any
deformation of the tube walls. How much would the diffusion flux increase with this reduction in thickness? On the
other hand, if the thickness determined in part (c) is found to be unsuitable, then specify a minimum thickness that
you would use. In this case, how much of a diminishment in diffusion flux would result?
Solution
(a) This portion of the problem asks for us to compute the wall thickness of a thin-walled cylindrical Ni tube
at 300°C through which hydrogen gas diffuses. The inside and outside pressures are, respectively, 1.1013 and
0.01013 MPa, and the diffusion flux is to be no greater than 1 ´ 10-7 mol/m2-s. This is a steady-state diffusion
problem, which necessitates that we employ Equation 5.3. The concentrations at the inside and outside wall faces
may be determined using Equation 6.28, and, furthermore, the diffusion coefficient is computed using Equation 6.29.
Solving for Dx (using Equation 5.3)
Dx = -
D DC
J
= -
(4.76
1
´
1 ´ 10 -7 mol/m2 - s
æ
ö
39, 560 J / mol
´ 10 -7 ) exp ç÷ ´
è (8.31 J/mol - K)(300 + 273 K ) ø
æ
ö
12, 300 J/mol
(30.8) expç÷
è (8.31 J/mol - K)(300 + 273 K ) ø
(
0.01013 MPa -
1.1013 MPa
)
= 0.0025 m = 2.5 mm
(b) Now we are asked to determine the circumferential stress:
s =
=
r Dp
4 Dx
(0.10 m)(1.013 MPa - 0.01013 MPa)
(4)(0.0025 m)
= 10.0 MPa
(c) Now we are to compare this value of stress to the yield strength of Ni at 300°C, from which it is possible
to determine whether or not the 2.5 mm wall thickness is suitable. From the information given in the problem, we may
write an equation for the dependence of yield strength (sy) on temperature (T) as follows:
s y = 100 MPa -
5 MPa
T - Tr
50°C
(
)
where Tr is room temperature and for temperature in degrees Celsius. Thus, at 300°C
s y = 100 MPa - (0.1 MPa/°C) (300°C - 20°C) = 72 MPa
Inasmuch as the circumferential stress (10 MPa) is much less than the yield strength (72 MPa), this thickness is
entirely suitable.
(d) And, finally, this part of the problem asks that we specify how much this thickness may be reduced and
still retain a safe design. Let us use a working stress by dividing the yield stress by a factor of safety, according to
Equation 6.24. On the basis of our experience, let us use a value of 2.0 for N. Thus
sw =
sy
N
=
72 MPa
= 36 MPa
2
Using this value for sw and Equation 6.30, we now compute the tube thickness as
Dx =
=
r Dp
4s w
(0.10 m)(1.013 MPa - 0.01013 MPa)
4(36 MPa)
= 0.00070 m = 0.70 mm
Substitution of this value into Fick's first law we calculate the diffusion flux as follows:
J = -D
DC
Dx
é
ù
39, 560 J/mol
= - (4.76 ´ 10 -7 ) exp êú ´
ë (8.31 J/mol - K)(300 + 273 K) û
é
ù
12, 300 J / mol
(30.8) exp êú 0.01013 MPa ë (8.31 J/mol - K)(300 + 273 K ) û
0.0007 m
(
1.013 MPa
)
= 3.53 ´ 10-7 mol/m2 -s
Thus, the flux increases by approximately a factor of 3.5, from 1 ´ 10-7 to 3.53 ´ 10-7 mol/m2-s with this reduction in
thickness.
6.D3 Consider the steady-state diffusion of hydrogen through the walls of a cylindrical nickel tube as
described in Problem 6.D2. One design calls for a diffusion flux of 5 ´ 10 -8 mol/m2-s, a tube radius of 0.125 m, and
inside and outside pressures of 2.026 MPa (20 atm) and 0.0203 MPa (0.2 atm), respectively; the maximum
allowable temperature is 450°C. Specify a suitable temperature and wall thickness to give this diffusion flux and
yet ensure that the tube walls will not experience any permanent deformation.
Solution
This problem calls for the specification of a temperature and cylindrical tube wall thickness that will give a
diffusion flux of 5 ´ 10-8 mol/m2-V IRUW
KH GLIIXVLRQ RI K\ GURJ HQ LQ QLFNHO W
KH W
XEH UDGLXVLV
P DQG W
KHLQVLGH
and outside pressures are 2.026 and 0.0203 MPa, respectively. There are probably several different approaches that
may be used; and, of course, there is not one unique solution. Let us employ the following procedure to solve this
problem: (1) assume some wall thickness, and, then, using Fick's first law for diffusion (which also employs
( TXDW
LRQV
DQG
FRP SXW
HW
KH W
HP SHUDW
XUH DWZKLFK W
KH GLIIXVLRQ IOX[ LV W
KDWUHTXLUHG
FRP SXW
HW
KH\ LHOG
strength of the nickel at this temperature using the dependence of yield strength on temperature as stated in Problem
'
FDOFXODW
HW
KH FLUFXP IHUHQW
LDOVW
UHVV RQ W
KH W
XEH ZDOOV XVLQJ ( TXDW
LRQ
DQG
FRP SDUH W
KH \ LHOG
strength and circumferential stress values--the yield strength should probably be at least twice the stress in order to
make certain that no permanent deformation occurs. If this condition is not met then another iteration of the
procedure should be conducted with a more educated choice of wall thickness.
As a starting point, let us arbitrarily choose a wall thickness of 2 mm (2 ´ 10-3 m). The steady-state
diffusion equation, Equation 5.3, takes the form
J = -D
DC
Dx
= 5 ´ 10-8 mol/m2-s
é
39, 560 J/mol ù
= - (4.76 ´ 10 -7 ) exp êú ´
ë (8.31 J/mol - K)(T) û
é
12, 300 J/mol ù
(30.8) exp êú 0.0203 MPa ë (8.31 J/mol - K)(T) û
0.002 m
(
2.026 MPa
)
Solving this expression for the temperature T gives T = 514 K = 241°C; this value is satisfactory inasmuch as it is less
than the maximum allowable value (450°C).
7 KHQH[WVW
HS LVW
R FRP SXW
HW
KHVW
UHVVRQ W
KHZDOOXVLQJ ( TXDW
LRQ
W
KXV
s =
=
r Dp
4 Dx
(0.125 m)(2.026 MPa - 0.0203 MPa)
(4) (2 ´ 10 -3 m)
= 31.3 MPa
Now, the yield strength (sy) of Ni at this temperature may be computed using the expression
s y = 100 MPa -
5 MPa
T - Tr
50°C
(
)
where Tr is room temperature. Thus,
sy = 100 MPa – (0.1 MPa/°C)(241°C – 20°C) = 77.9 MPa
Inasmuch as this yield strength is greater than twice the circumferential stress, wall thickness and temperature values
of 2 mm and 241°C are satisfactory design parameters.
```